TECHBRIEF Improved Corrosion-
Resistant Steel for Highway
FHWA Publication No.: FHWA HRT-09-053
FHWA Contact: Y. Paul Virmani, HRDI-10, (202) 493-3052,
The use of weathering steels for construction of new high-
way bridges has recently increased significantly. These
steels provide construction cost savings of more than
10 percent because there is no need to paint the steel, as
unpainted steel is easier to install and handle. In addition,
the life-cycle cost savings are more than 30 percent because
weathering steels require less maintenance and are more
durable than common construction steels. Also, use of weather-
ing steels provides significant environmental benefits because
there are no volatile organic compounds (VOC) from paints,
and there is no need for removal or disposal of contaminated
blast debris over the life span of the structure. However, the
current weathering steels are not considered adequate for
marine and other high saline environments. The objective
of this project was to point out new directions for the devel-
opment of low-cost steels with much better weathering charac-
teristics than those of currently used weathering steels.
This project did not involve experimental laboratory or field
tests of weathering steels. Instead, it focused on an extensive
analysis of available data regarding the weathering perfor-
mance of steels in different environments, effects of different
conventional and nonconventional alloying elements on
weathering of steels, and mechanisms leading to the reduced
Research, Development, and corrosion rates of those steels with the goal of suggesting ways
Technology to improve the weathering characteristics of modified existing
Turner-Fairbank Highway steels. Prior design of weathering steels was purely empirical,
Research Center and the steel design focus was on a small number of conventional
6300 Georgetown Pike elements such as manganese (Mn), silicon (Si), chromium (Cr),
nickel (Ni), copper (Cu), molybdenum (Mo), and phosphorus
McLean, VA 22101-2296
(P) in a narrow concentration range. Since the effects of these
elements on corrosion properties of steels were well known
www.tfhrc.gov for many decades, only marginal improvement in weather-
ing performance of steels could be achieved by adjusting the
concentrations of these elements.
With the increased use of thermodynamics (i.e. high values of pH. Thus, Cr is more effective
Pourbaix diagrams), electrochemical impedance in corrosion protection of Fe than Ni.
spectroscopy (EIS), X-ray diffraction (XRD), and
Mössbauer spectroscopy in the corrosion field, it • When W is added to Fe, the anion (WO4)-2
became obvious that there might be several dif- is formed at pH as low as 5.(3) This anion,
ferent mechanisms for imparting corrosion resis- when combined with the Fe cation during
tance to weathering steels depending on the early stages of weathering, forms a salt that
nature of the alloying element and on the environ- concentrates in the pores of the rust and acts
ment. Thus, better understanding the corrosion as a corrosion inhibitor. No ions are formed
mechanisms led to a significant extension of the at high pH values in Fe-W systems. Thus,
list of possible alloying elements that improve this alloy is also passive at high pHs.
the weatherability of steel. Discussion below sug-
• When Al is added to Fe, a stable FeAl2O4
gests that more significant increases in weather-
protective oxide forms in a wide pH region
ing performance of steels could be achieved by
(from 4 to 14).(3)
using less common alloying elements such as
tungsten (W), titanium (Ti), aluminum (Al), rare Since no information on corrosion kinetics
earths (RE), etc., than by using traditional alloy- could be deduced from Pourbaix diagrams,
ing elements. These suggestions are based on further analysis of the effects of these elements
the laboratory-performed accelerated weath- on morphology and electrical (impedance) resis-
ering tests as well as on studies of the effects tance of the films formed on the surfaces of
of these elements on thermodynamic, kinetic, steels that have been performed by other
electrochemical, crystallographic, and other prop- analytical techniques were reviewed to ascertain
erties of native oxide layers on steels. whether the addition of these elements impr-
oved the weatherability of steel.
The rust on steel is a semiconductor; therefore,
Since the corrosion process is electrochemical the direct measurement of electrical resistance
by nature, the electrical potential of the system of it is not possible. Instead, EIS has been
and pH of the environment are very important successfully applied to the study of corrosion
factors in the weathering of steels. Pourbaix dia- systems for many decades and has been proven
grams, also known as potential/pH diagrams, to be a powerful and accurate method for
map out possible stable equilibrium phases of an measuring corrosion rates. For example, when
aqueous electrochemical system.(1) Weathering of EIS was used to determine the resistivity of
steel depends on the formation of a hard passive the oxides on the surface of binary alloys, the
surface film (oxide or salt) that inhibits further highest resistance of the rust was observed
corrosion. The Pourbaix diagram indicates that when 1 percent of W was added to Fe.(4) The
pure iron is passive at pH values from 9 to 12.5 resistance of the rust formed on Fe with
(iron hydroxide forms in this pH range).(1) Below 1 percent W was one order of magnitude higher
or above this pH range, iron corrodes freely. than that of the rusts formed on Fe with an
Pourbaix diagrams for binary systems (iron-other addition of 3 percent cobalt (Co), 0.1 percent P ,
elements) or ternary (iron-two other elements) or 0.8 percent Al. In addition, the resistance
calculated at Northwestern University and other was a few times higher than that of rust
research groups showed the following: formed on steel containing 0.8 percent Mo or
3 percent Ni. According to the American Society
• When Ni is added, it prevents the corrosion for Testing and Materials (ASTM)’s Volume
of iron (Fe) at a pH higher than 12.5 by 03.02, Wear and Erosion: Metal Testing, Co, P,
the formation of a stable oxide. In addition, Mo, and Ni are very potent in making steel
Ni extends the passive region down to weatherable.(5) Thus, on the basis of EIS results,
pH 7.(2) Formation of the spinel double oxide it could be anticipated that W would be an
(NiFe2O4) on the steel during weathering even more potent element than others in the
provides an additional measure of protection weathering of steels.
from further corrosion.
Another recent research of the steels contain-
• When Cr is added to Fe, the passive region ing Al confirmed the conclusions made from
is extended further than in case of Ni down Pourbaix diagram analysis.(6) The addition of
to pH equal to 4.5, and no ions are formed at 0.8 percent Al to steel almost doubled the
impedance of the rust compared to similar steel As demonstrated before, less common alloying
without Al. This further suggests that Al could elements in steel (Al, Ti, W, and REs) can signifi-
significantly improve the weatherability of steels. cantly affect the steel weatherability. The addition
of any of these elements or their combination
The addition of another element, Ti, to the steel
would not significantly affect the price of steel
leads to a modification of the rust morphology (as
because these elements are inexpensive when
found by transmission electron microscopy (TEM)
added in small amounts. The mechanical prop-
and characterized by XRD, nitrogen (N2) absorp-
erties of steel were shown to be improved by
tion, and Mössbauer spectroscopy).(7) Ti-enriched the addition of some of these elements. For
ultrafine α-FeOOH particles plug the pores in the example, the addition of REs to steel refined
rust film formed on the steel surface, which sig- the microstructure, increased the strength, and
nificantly increases the passivation ability of the rust. increased fracture toughness. Furthermore, the
Another benefit of small Ti addition is its ability to use of Al in steel increased its strength and did
suppress the formation of pearlite in steel, improv- not affect the toughness. Meanwhile, the use
ing the weatherability of steel.(8) Steel that con- of Ti refined the microstructure, eliminated pearl-
tains pearlite has significantly lower weatherability ite, and dramatically increased fracture tough-
than steel of the same composition but with the ness at cryogenic temperatures.
C in solution in the ferrite.(9)
Based on these findings, an experimental
It was found that very small additions of RE
approach is suggested to design a more effective
elements to steel significantly improve its weath-
weathering steel based on an ASTM A710
erability. In one investigation, it was found that
Grade B steel developed at Northwestern Univ-
after 2,250 days of outdoor exposure, the cor-
rosion rate of steel that contained a very small ersity.(11,12) This 70-ksi yield steel has excell-
addition of RE elements (0.029 percent) was two ent ductility, fracture toughness, weldability,
times less than that of the steel without these machinability, and weatherability that is sup-
elements.(10) The addition of these elements erior to the properties of other weather-
moved the corrosion potential of the steel in a ing steels presently used for bridges. The foll-
positive direction as well as significantly increa- owing elements are proposed to be added to the
sed the electrical resistance of the rust layer. steel separately: Al in 0.2–0.8 percent, Ti in
These results showed that the addition of REs 0.1–1.0 percent, RE elements in 0.01–0.05 percent,
of proper proportion may significantly diminish and W in 0.3–1.0 percent. The mechanical and
corrosion tendency and promote the formation fracture properties should be tested. If they
of the steady and compact rust layer. conform to bridge steel requirements, the weath-
erability of steel should be investigated in accel-
While corrosion resistance is an important erated tests. Additional steel compositions that
performance factor for steels, other factors need include the combination of two or more of these
to be considered in the design of improved elements could be designed after the preliminary
weathering steels. These factors include mech- mechanical, fracture, and corrosion tests are
anical properties such as strength, ductility, and performed, and the beneficial effects of these
high fracture resistance at low temperatures; elements on steel properties are ascertained.
the ability of steel companies to produce steel
through steel-making processes; the ease of
steel structure fabrication such as weldability
and machinability; the absence of adverse Based on research performed by different
health effects during steel production and struc- groups and on work performed at Northwestern
ture fabrication; reasonable cost; etc. For University, it is found that many of the less
example, P is very effective in increasing the used elements in steel such as Al, Ti, W, and
weatherability of steel; however, in amounts REs could significantly improve the weathera-
exceeding 0.1 percent, it significantly imbrittles bility of steel.
the steel. Elements Cr and Mn are very effective
for weatherability, but steels containing these Weathering steel could not be designed solely
elements release carcinogenic fumes during on its weathering characteristics. The composi-
welding. As a result, the concentration of these tion should be optimized in respect to weathering
elements in steel needs to be kept to a minimum. characteristics, strength, ductility and fracture
However, the element Mo is very expensive and properties, ease of processing and fabrication,
should be avoided if possible. cost, and adverse health effects.
Further experimental work is recommended. 7. Nakayama, T., Ishikawa, T., and Konno, T.J.
For example, an improved corrosion-resistant (2005). “Structure of Titanium-Doped Goethite
steel could be designed by modification of ”
Rust, Corrosion Science, 47, 2521.
ASTM A710 Grade B steel composition by the
addition of Ti, Al, P W, RE elements, and other
, 8. Vaynman, S. et al. Effect of Ti on Charpy
elements not usually found in steels. Fracture Energy and Other Mechanical
Properties of ASTM A 710 Grade B Cu-
Precipitation-Strengthened Steel. To be
published in 2009.
1. Pourbaix, M. (1966). Atlas of Electrochemical
Equilibria in Aqueous Solutions, Pergamon 9. Zhao, Y.T. et al. (2007). “The Mechanical
Press, Brussels, Belgium. Properties and Corrosion Behaviors of Ultra-
Low Carbon Microalloying Steel, Materials
2. Nishimura, T. and Kodama, T. (2003).
Science and Engineering A: Structural
“Clarification of Chemical State for Alloying
Materials Properties Microstructure and
Elements in Iron Rust Using a Binary-Phase
Processing, 454, 695.
Potential–pH Diagram and Physical Analyses, ”
Corrosion Science, 45, 1073. 10. Wang, L.M. et al. (2008). “New Study
3. Hara, S. et al. (2007). “Taxonomy for Prot- Concerning Development of Application of
ective Ability of Rust Layer Using its ”
Rare Earth Metals in Steels, Journal of Alloys
Composition Formed on Weathering Steel and Compounds, 45l, 534.
Bridge, Corrosion Science, 49, 1131.
11. Vaynman, S. , Fine, M.E., and Bhat, S.P (2004).
4. Itagaki, M. et al. (2004). “Electrochemical “High-Strength, Low-Carbon, Ferritic, Copper-
Impedance of Thin Rust Film of Low-Alloy Precipitation-Strengthening Steels for Tank
Steels, Corrosion Science, 46, 1301. ”
Car Applications, Materials Science and
5. ASTM International Standards. (2004). Wear Technology 2004 Conference Proceedings,
and Erosion: Metal Testing, Vol. 03.02, West AIST and TMS, 417, New Orleans, LA.
12. Vaynman, S. et al. (2002). “High Perfor-
6. Nishimura, T. (2008). “Corrosion Resistance mance Copper-Precipitation-Hardened Steel, ”
of Si–Al-Bearing Ultrafine-Grained Weathering Microalloyed Steels, ASM International, 43.
Steel, Science and Technology of Advanced
Researchers—This study was performed by Northwestern University, Department of Materials Science and
Engineering, 2220 N. Campus Drive, Evanston, IL 60208, (847) 491-4475.
Distribution—This TechBrief is being distributed according to a standard distribution. Direct
distribution is being made to the Divisions and Resource Center.
Availability— The TechBrief may be obtained from the FHWA Product Distribution Center by e-mail to
Report.Center@dot.gov, fax to (814) 239-2156, phone to (814) 239-1160, or online at http://www.tfhrc.gov/structur/pubs.htm.
Key Words— Alloying element, Pourbaix diagram, Steel, Chloride ions, and Weatherability.
Notice—This document is disseminated under the sponsorship of the U.S. Department of Transportation in the in-
terest of information exchange. The U.S. Government assumes no liability for the use of the information contained
in this document. The U.S. Government does not endorse products or manufacturers. Trademarks or manufacturers’
names appear in this report only because they are considered essential to the objective of the document.
Quality Assurance Statement—The Federal Highway Administration (FHWA) provides high-quality information
to serve the Government, industry, and public in a manner that promotes public understanding. Standards and poli-
cies are used to ensure and maximize the quality, objectivity, utility, and integrity of its information. FHWA periodi-
cally reviews quality issues and adjusts its programs and
processes to ensure continuous quality improvement.
AUGUST 2009 FHWA-HRT-09-053